#------------------------------------------------------------------------------
#$Date: 2018-10-05 15:19:55 +0300 (Fri, 05 Oct 2018) $
#$Revision: 211332 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/31/57/4315778.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4315778
loop_
_publ_author_name
'David L. Rogow'
'Honghan Fei'
'Daniel P. Brennan'
'Mariko Ikehata'
'Peter Y. Zavalij'
'Allen G. Oliver'
'Scott R. J. Oliver'
_publ_contact_author_address     '258 PSB'
_publ_contact_author_email       soliver@chemistry.ucsc.edu
_publ_contact_author_name        'Scott Oliver'
_publ_contact_author_phone       9-5448
_publ_section_title
;
 Hydrothermal Synthesis of Two Cationic Bismuthate Clusters: An
 Alkylenedisulfonate Bridged Hexamer, [Bi6O4(OH)4(H2O)2][(CH2)2(SO3)2]3
 and a Rare Nonamer Templated by Triflate, [Bi9O8(OH)6][CF3SO3]5
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              5619
_journal_page_last               5624
_journal_paper_doi               10.1021/ic1004402
_journal_volume                  49
_journal_year                    2010
_chemical_formula_moiety         'Bi9 O14, 5(C F3 O3 S)'
_chemical_formula_sum            'C5 Bi9 F15 O29 S5'
_chemical_formula_weight         2850.17
_chemical_name_common            'trifluoromethylsolfonate bismuth oxide'
_chemical_name_systematic
;
pentakis-trifluoromethylsolfonate nonabismuth tetradecaoxide
;
_space_group_IT_number           15
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_atom_sites_solution_hydrogens   undef
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           'SHELXL-97 & ZCIF'
_cell_angle_alpha                90.00
_cell_angle_beta                 99.665(7)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   17.463(6)
_cell_length_b                   10.114(4)
_cell_length_c                   23.924(9)
_cell_measurement_reflns_used    4811
_cell_measurement_temperature    299(2)
_cell_measurement_theta_max      31.0
_cell_measurement_theta_min      2.3
_cell_volume                     4166(3)
_computing_cell_refinement       'SAINT (Bruker, 1999)'
_computing_data_collection       'SMART (Bruker, 1999)'
_computing_data_reduction        SAINT
_computing_molecular_graphics    'ORTEP-3 (Farrugia,1997), ATOMS (Dowty,1999)'
_computing_publication_material  SHELXL-97
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      299(2)
_diffrn_detector                 'CCD area detector'
_diffrn_detector_area_resol_mean 8.33
_diffrn_detector_type            'Bruker SmartApex'
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_details      NFRAMES=606,606,606,50,1206,50
_diffrn_measurement_device_type  'three-circle diffractometer'
_diffrn_measurement_method       'ω scans'
_diffrn_measurement_specimen_support 'glass capillary'
_diffrn_orient_matrix_type       standard
_diffrn_orient_matrix_UB_11      0.0504448
_diffrn_orient_matrix_UB_12      0.0464910
_diffrn_orient_matrix_UB_13      -0.0004523
_diffrn_orient_matrix_UB_21      0.0136726
_diffrn_orient_matrix_UB_22      -0.0106860
_diffrn_orient_matrix_UB_23      0.0420443
_diffrn_orient_matrix_UB_31      0.0253517
_diffrn_orient_matrix_UB_32      -0.0866021
_diffrn_orient_matrix_UB_33      -0.0054649
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0666
_diffrn_reflns_av_sigmaI/netI    0.0701
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -31
_diffrn_reflns_number            23984
_diffrn_reflns_theta_full        28.28
_diffrn_reflns_theta_max         28.28
_diffrn_reflns_theta_min         2.37
_diffrn_source_current           30
_diffrn_source_voltage           50
_diffrn_standards_decay_%        0.15
_exptl_absorpt_coefficient_mu    38.279
_exptl_absorpt_correction_T_max  0.563
_exptl_absorpt_correction_T_min  0.067
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'XPREP (Sheldrick, 1997)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    4.545
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             4896
_exptl_crystal_id                'Dan/Scott B2O3+F3CSO3H+NH4OH Crystal#3'
_exptl_crystal_size_max          0.310
_exptl_crystal_size_mid          0.145
_exptl_crystal_size_min          0.015
_refine_diff_density_max         2.335
_refine_diff_density_min         -1.248
_refine_diff_density_rms         0.298
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.000
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     325
_refine_ls_number_reflns         5161
_refine_ls_number_restraints     105
_refine_ls_restrained_S_all      1.028
_refine_ls_R_factor_all          0.0628
_refine_ls_R_factor_gt           0.0382
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0115P)²], P=(max(Fo²,0)+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0567
_refine_ls_wR_factor_ref         0.0596
_reflns_number_gt                3573
_reflns_number_total             5161
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic1004402_si_003.cif
_cod_data_source_block           SLUG-16
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Monoclinic' changed to 'monoclinic'
according to the built-in table from CIF Core dictionary named
'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 
;
_cod_database_code               4315778
_diffrn_measurement_total_frames-ccd 3124
_diffrn_measurement_frame_width-ccd 0.3
_diffrn_detector_distance-ccd    5.156
_diffrn_measurement_frame_time-ccd 10
_diffrn_measurement_total_time-ccd 11.72
_diffrn_measurement_frame_size-ccd 512
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x, -y, z-1/2'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Bi1 Bi 0.41092(2) 0.45396(4) 0.32674(2) 0.02756(11) Uani 1 1 d . . .
Bi2 Bi 0.37480(2) 0.45389(4) 0.17495(2) 0.02861(12) Uani 1 1 d . . .
Bi3 Bi 0.48214(2) 0.77544(4) 0.17415(2) 0.02813(11) Uani 1 1 d . . .
Bi4 Bi 0.5000 0.19161(6) 0.2500 0.03293(17) Uani 1 2 d S . .
Bi5 Bi 0.31519(2) 0.74629(4) 0.25050(2) 0.03350(12) Uani 1 1 d . . .
O1 O 0.5153(3) 0.5617(6) 0.3160(3) 0.0256(18) Uani 1 1 d . . .
O2 O 0.4147(3) 0.3385(6) 0.2499(3) 0.0257(17) Uani 1 1 d . . .
O3 O 0.4785(4) 0.2885(7) 0.1603(3) 0.037(2) Uani 1 1 d . . .
O4 O 0.3447(4) 0.5463(6) 0.2505(3) 0.0333(19) Uani 1 1 d . . .
O5 O 0.3867(3) 0.6974(6) 0.3405(3) 0.0296(19) Uani 1 1 d . . .
O6 O 0.3416(4) 0.6990(7) 0.1607(3) 0.036(2) Uani 1 1 d . . .
O7 O 0.4304(4) 0.8010(6) 0.2503(3) 0.0306(19) Uani 1 1 d . . .
S1 S 0.35793(15) 0.0612(3) 0.34943(15) 0.0347(8) Uani 1 1 d D . .
O11 O 0.4335(4) 0.0293(7) 0.3370(4) 0.057(3) Uani 1 1 d D . .
O12 O 0.2990(4) -0.0344(7) 0.3308(4) 0.060(3) Uani 1 1 d D . .
O13 O 0.3329(4) 0.1955(7) 0.3393(4) 0.058(3) Uani 1 1 d D . .
C1 C 0.3690(9) 0.0445(16) 0.4237(11) 0.134(10) Uani 1 1 d D . .
F11 F 0.3014(7) 0.0820(13) 0.4393(5) 0.157(5) Uani 1 1 d D . .
F12 F 0.4242(8) 0.1225(16) 0.4480(6) 0.217(9) Uani 1 1 d D . .
F13 F 0.3884(9) -0.0732(13) 0.4403(5) 0.189(7) Uani 1 1 d D . .
S2 S 0.18999(15) 0.5636(3) 0.34963(15) 0.0346(8) Uani 1 1 d D . .
O21 O 0.2443(4) 0.4639(7) 0.3394(4) 0.056(3) Uani 1 1 d D . .
O22 O 0.1115(4) 0.5311(8) 0.3312(4) 0.064(3) Uani 1 1 d D . .
O23 O 0.2100(4) 0.6960(7) 0.3365(4) 0.055(3) Uani 1 1 d D . .
C2 C 0.1948(11) 0.5634(16) 0.4258(10) 0.115(8) Uani 1 1 d D . .
F21 F 0.1413(9) 0.6456(15) 0.4366(5) 0.196(7) Uani 1 1 d D . .
F23 F 0.1823(9) 0.4435(12) 0.4417(5) 0.186(7) Uani 1 1 d D . .
F22 F 0.2637(10) 0.6001(15) 0.4479(6) 0.230(9) Uani 1 1 d D . .
S3 S 0.4919(8) 0.5842(15) 0.0238(6) 0.175(6) Uani 0.50 1 d PDU . .
O31 O 0.4612(14) 0.6973(18) 0.0528(9) 0.117(9) Uani 0.50 1 d PDU . .
O32 O 0.5322(12) 0.482(2) 0.0583(8) 0.108(8) Uani 0.50 1 d PDU . .
O33 O 0.5268(14) 0.615(2) -0.0244(9) 0.148(11) Uani 0.50 1 d PDU . .
C3 C 0.3983(18) 0.519(2) 0.0040(10) 0.32(5) Uani 0.50 1 d PDU . .
F31 F 0.3588(12) 0.618(2) -0.0253(10) 0.164(10) Uani 0.50 1 d PDU . .
F32 F 0.3730(11) 0.503(2) 0.0524(8) 0.128(8) Uani 0.50 1 d PDU . .
F33 F 0.3922(18) 0.406(3) -0.0207(14) 0.36(3) Uani 0.50 1 d PDU . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Bi Bi -4.1077 10.2566 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Bi1 O2 91.3(2) . . ?
O1 Bi1 O4 91.3(2) . . ?
O2 Bi1 O4 67.4(2) . . ?
O1 Bi1 O5 71.9(2) . . ?
O2 Bi1 O5 131.2(2) . . ?
O4 Bi1 O5 67.5(2) . . ?
O1 Bi1 O3 73.1(2) . 2_655 ?
O2 Bi1 O3 67.7(2) . 2_655 ?
O4 Bi1 O3 131.8(3) . 2_655 ?
O5 Bi1 O3 140.1(2) . 2_655 ?
O1 Bi1 O32 84.2(4) . 2_655 ?
O2 Bi1 O32 146.0(5) . 2_655 ?
O4 Bi1 O32 146.1(5) . 2_655 ?
O5 Bi1 O32 79.2(5) . 2_655 ?
O3 Bi1 O32 78.9(5) 2_655 2_655 ?
O1 Bi1 O21 148.0(2) . . ?
O2 Bi1 O21 105.7(2) . . ?
O4 Bi1 O21 71.5(2) . . ?
O5 Bi1 O21 76.50(19) . . ?
O3 Bi1 O21 138.4(2) 2_655 . ?
O32 Bi1 O21 95.1(5) 2_655 . ?
O1 Bi1 O13 148.8(2) . . ?
O2 Bi1 O13 72.3(2) . . ?
O4 Bi1 O13 105.7(2) . . ?
O5 Bi1 O13 138.62(19) . . ?
O3 Bi1 O13 76.1(2) 2_655 . ?
O32 Bi1 O13 94.7(4) 2_655 . ?
O21 Bi1 O13 63.20(19) . . ?
O2 Bi2 O4 68.3(2) . . ?
O2 Bi2 O1 91.8(2) . 2_655 ?
O4 Bi2 O1 91.9(2) . 2_655 ?
O2 Bi2 O3 67.6(2) . . ?
O4 Bi2 O3 132.6(3) . . ?
O1 Bi2 O3 73.0(2) 2_655 . ?
O2 Bi2 O6 132.1(2) . . ?
O4 Bi2 O6 67.2(2) . . ?
O1 Bi2 O6 72.9(2) 2_655 . ?
O3 Bi2 O6 140.7(2) . . ?
O2 Bi2 F32 149.4(4) . . ?
O4 Bi2 F32 141.7(5) . . ?
O1 Bi2 F32 83.0(4) 2_655 . ?
O3 Bi2 F32 82.1(4) . . ?
O6 Bi2 F32 75.1(5) . . ?
O2 Bi2 O23 71.9(2) . 4_545 ?
O4 Bi2 O23 105.4(2) . 4_545 ?
O1 Bi2 O23 149.0(2) 2_655 4_545 ?
O3 Bi2 O23 76.4(2) . 4_545 ?
O6 Bi2 O23 137.4(2) . 4_545 ?
F32 Bi2 O23 97.6(5) . 4_545 ?
O2 Bi2 O12 104.0(2) . 4 ?
O4 Bi2 O12 68.9(3) . 4 ?
O1 Bi2 O12 147.6(2) 2_655 4 ?
O3 Bi2 O12 139.2(2) . 4 ?
O6 Bi2 O12 75.6(2) . 4 ?
F32 Bi2 O12 96.0(4) . 4 ?
O23 Bi2 O12 63.3(2) 4_545 4 ?
O1 Bi3 O7 91.7(2) 2_655 2_655 ?
O1 Bi3 O7 91.8(2) 2_655 . ?
O7 Bi3 O7 67.9(3) 2_655 . ?
O1 Bi3 O5 72.5(2) 2_655 2_655 ?
O7 Bi3 O5 67.8(2) 2_655 2_655 ?
O7 Bi3 O5 132.2(2) . 2_655 ?
O1 Bi3 O6 73.3(2) 2_655 . ?
O7 Bi3 O6 132.0(3) 2_655 . ?
O7 Bi3 O6 67.4(2) . . ?
O5 Bi3 O6 140.7(2) 2_655 . ?
O1 Bi3 O31 80.7(4) 2_655 . ?
O7 Bi3 O31 142.8(5) 2_655 . ?
O7 Bi3 O31 148.0(5) . . ?
O5 Bi3 O31 75.2(5) 2_655 . ?
O6 Bi3 O31 80.7(5) . . ?
O1 Bi3 O11 149.4(2) 2_655 2_665 ?
O7 Bi3 O11 71.6(2) 2_655 2_665 ?
O7 Bi3 O11 104.6(2) . 2_665 ?
O5 Bi3 O11 77.42(19) 2_655 2_665 ?
O6 Bi3 O11 136.8(2) . 2_665 ?
O31 Bi3 O11 97.0(5) . 2_665 ?
O1 Bi3 O22 148.0(2) 2_655 4 ?
O7 Bi3 O22 103.3(2) 2_655 4 ?
O7 Bi3 O22 68.9(3) . 4 ?
O5 Bi3 O22 139.3(2) 2_655 4 ?
O6 Bi3 O22 75.7(2) . 4 ?
O31 Bi3 O22 102.0(4) . 4 ?
O11 Bi3 O22 62.48(19) 2_665 4 ?
O2 Bi4 O2 90.1(4) 2_655 . ?
O2 Bi4 O3 72.4(2) 2_655 2_655 ?
O2 Bi4 O3 73.0(2) . 2_655 ?
O2 Bi4 O3 73.0(2) 2_655 . ?
O2 Bi4 O3 72.4(2) . . ?
O3 Bi4 O3 130.3(3) 2_655 . ?
O2 Bi4 O22 140.2(3) 2_655 4_545 ?
O2 Bi4 O22 90.0(2) . 4_545 ?
O3 Bi4 O22 144.4(2) 2_655 4_545 ?
O3 Bi4 O22 69.1(2) . 4_545 ?
O2 Bi4 O22 90.0(2) 2_655 3_545 ?
O2 Bi4 O22 140.2(3) . 3_545 ?
O3 Bi4 O22 69.1(2) 2_655 3_545 ?
O3 Bi4 O22 144.4(2) . 3_545 ?
O22 Bi4 O22 114.2(3) 4_545 3_545 ?
O2 Bi4 O11 137.3(3) 2_655 . ?
O2 Bi4 O11 91.7(2) . . ?
O3 Bi4 O11 67.5(2) 2_655 . ?
O3 Bi4 O11 147.0(2) . . ?
O22 Bi4 O11 82.5(2) 4_545 . ?
O22 Bi4 O11 62.8(2) 3_545 . ?
O2 Bi4 O11 91.7(2) 2_655 2_655 ?
O2 Bi4 O11 137.3(3) . 2_655 ?
O3 Bi4 O11 147.0(2) 2_655 2_655 ?
O3 Bi4 O11 67.5(2) . 2_655 ?
O22 Bi4 O11 62.8(2) 4_545 2_655 ?
O22 Bi4 O11 82.5(2) 3_545 2_655 ?
O11 Bi4 O11 114.4(3) . 2_655 ?
O4 Bi5 O7 91.1(2) . . ?
O4 Bi5 O6 73.3(3) . . ?
O7 Bi5 O6 73.2(3) . . ?
O4 Bi5 O5 72.8(3) . . ?
O7 Bi5 O5 72.2(3) . . ?
O6 Bi5 O5 130.3(2) . . ?
O4 Bi5 O12 140.5(3) . 1_565 ?
O7 Bi5 O12 90.0(2) . 1_565 ?
O6 Bi5 O12 143.7(2) . 1_565 ?
O5 Bi5 O12 70.1(2) . 1_565 ?
O4 Bi5 O23 90.9(2) . . ?
O7 Bi5 O23 137.9(3) . . ?
O6 Bi5 O23 146.4(2) . . ?
O5 Bi5 O23 68.4(2) . . ?
O12 Bi5 O23 63.4(2) 1_565 . ?
Bi3 O1 Bi1 119.2(3) 2_655 . ?
Bi3 O1 Bi2 118.9(3) 2_655 2_655 ?
Bi1 O1 Bi2 118.5(3) . 2_655 ?
Bi4 O2 Bi2 120.9(3) . . ?
Bi4 O2 Bi1 119.8(3) . . ?
Bi2 O2 Bi1 111.0(3) . . ?
Bi4 O3 Bi2 99.1(3) . . ?
Bi4 O3 Bi1 99.4(3) . 2_655 ?
Bi2 O3 Bi1 95.4(2) . 2_655 ?
Bi5 O4 Bi2 120.7(3) . . ?
Bi5 O4 Bi1 120.5(3) . . ?
Bi2 O4 Bi1 109.9(3) . . ?
Bi5 O5 Bi3 99.4(3) . 2_655 ?
Bi5 O5 Bi1 99.2(3) . . ?
Bi3 O5 Bi1 96.4(2) 2_655 . ?
Bi5 O6 Bi3 99.0(3) . . ?
Bi5 O6 Bi2 98.8(3) . . ?
Bi3 O6 Bi2 94.9(2) . . ?
Bi5 O7 Bi3 120.6(3) . 2_655 ?
Bi5 O7 Bi3 120.3(3) . . ?
Bi3 O7 Bi3 110.4(3) 2_655 . ?
O12 S1 O13 113.9(5) . . ?
O12 S1 O11 115.0(5) . . ?
O13 S1 O11 116.2(5) . . ?
O12 S1 C1 101.6(7) . . ?
O13 S1 C1 103.8(6) . . ?
O11 S1 C1 103.8(6) . . ?
F13 C1 F12 106.5(18) . . ?
F13 C1 F11 111.9(16) . . ?
F12 C1 F11 108.8(17) . . ?
F13 C1 S1 112.3(15) . . ?
F12 C1 S1 109.8(15) . . ?
F11 C1 S1 107.4(14) . . ?
O22 S2 O23 114.3(5) . . ?
O22 S2 O21 114.8(5) . . ?
O23 S2 O21 115.3(5) . . ?
O22 S2 C2 101.1(7) . . ?
O23 S2 C2 104.5(7) . . ?
O21 S2 C2 104.5(7) . . ?
F22 C2 F23 109.9(17) . . ?
F22 C2 F21 112.6(19) . . ?
F23 C2 F21 112.0(16) . . ?
F22 C2 S2 107.1(15) . . ?
F23 C2 S2 108.4(15) . . ?
F21 C2 S2 106.5(14) . . ?
O33 S3 O32 112.8(14) . . ?
O33 S3 O31 116.6(15) . . ?
O32 S3 O31 118.0(14) . . ?
O33 S3 C3 111.6(14) . . ?
O32 S3 C3 103.2(13) . . ?
O31 S3 C3 91.4(13) . . ?
F33 C3 F32 106(2) . . ?
F33 C3 F31 115(2) . . ?
F32 C3 F31 109(2) . . ?
F33 C3 S3 117(2) . . ?
F32 C3 S3 104.1(19) . . ?
F31 C3 S3 103.6(19) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Bi1 O1 2.176(6) . ?
Bi1 O2 2.187(7) . ?
Bi1 O4 2.198(7) . ?
Bi1 O5 2.529(6) . ?
Bi1 O3 2.535(7) 2_655 ?
Bi1 O32 2.776(19) 2_655 ?
Bi1 O21 2.977(7) . ?
Bi1 O13 2.986(7) . ?
Bi2 O2 2.156(7) . ?
Bi2 O4 2.176(7) . ?
Bi2 O1 2.186(6) 2_655 ?
Bi2 O3 2.533(6) . ?
Bi2 O6 2.555(7) . ?
Bi2 F32 2.969(18) . ?
Bi2 O23 2.990(7) 4_545 ?
Bi2 O12 3.017(7) 4 ?
Bi3 O1 2.175(6) 2_655 ?
Bi3 O7 2.177(7) 2_655 ?
Bi3 O7 2.180(7) . ?
Bi3 O5 2.502(6) 2_655 ?
Bi3 O6 2.542(6) . ?
Bi3 O31 2.97(2) . ?
Bi3 O11 2.994(7) 2_665 ?
Bi3 O22 3.051(8) 4 ?
Bi4 O2 2.104(6) 2_655 ?
Bi4 O2 2.104(6) . ?
Bi4 O3 2.330(8) 2_655 ?
Bi4 O3 2.330(8) . ?
Bi4 O22 2.989(9) 4_545 ?
Bi4 O22 2.989(9) 3_545 ?
Bi4 O11 3.032(8) . ?
Bi4 O11 3.032(8) 2_655 ?
Bi5 O4 2.087(6) . ?
Bi5 O7 2.088(6) . ?
Bi5 O6 2.322(8) . ?
Bi5 O5 2.353(7) . ?
Bi5 O12 2.980(8) 1_565 ?
Bi5 O23 3.023(8) . ?
S1 O12 1.427(7) . ?
S1 O13 1.435(7) . ?
S1 O11 1.437(6) . ?
S1 C1 1.76(3) . ?
C1 F13 1.282(15) . ?
C1 F12 1.305(15) . ?
C1 F11 1.350(14) . ?
S2 O22 1.406(7) . ?
S2 O23 1.431(7) . ?
S2 O21 1.434(7) . ?
S2 C2 1.81(2) . ?
C2 F22 1.285(16) . ?
C2 F23 1.301(15) . ?
C2 F21 1.308(15) . ?
S3 O33 1.426(13) . ?
S3 O32 1.434(12) . ?
S3 O31 1.484(12) . ?
S3 C3 1.75(3) . ?
C3 F33 1.286(17) . ?
C3 F32 1.316(17) . ?
C3 F31 1.343(16) . ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 Bi1 O1 Bi3 134.1(4) . . . 2_655 ?
O4 Bi1 O1 Bi3 66.7(4) . . . 2_655 ?
O5 Bi1 O1 Bi3 0.9(3) . . . 2_655 ?
O3 Bi1 O1 Bi3 -159.7(4) 2_655 . . 2_655 ?
O32 Bi1 O1 Bi3 -79.6(6) 2_655 . . 2_655 ?
O21 Bi1 O1 Bi3 10.8(7) . . . 2_655 ?
O13 Bi1 O1 Bi3 -169.2(4) . . . 2_655 ?
O2 Bi1 O1 Bi2 -67.0(4) . . . 2_655 ?
O4 Bi1 O1 Bi2 -134.4(4) . . . 2_655 ?
O5 Bi1 O1 Bi2 159.8(4) . . . 2_655 ?
O3 Bi1 O1 Bi2 -0.8(3) 2_655 . . 2_655 ?
O32 Bi1 O1 Bi2 79.3(6) 2_655 . . 2_655 ?
O21 Bi1 O1 Bi2 169.7(3) . . . 2_655 ?
O13 Bi1 O1 Bi2 -10.2(7) . . . 2_655 ?
O2 Bi4 O2 Bi2 72.9(3) 2_655 . . . ?
O3 Bi4 O2 Bi2 144.4(4) 2_655 . . . ?
O3 Bi4 O2 Bi2 0.7(3) . . . . ?
O22 Bi4 O2 Bi2 -67.3(4) 4_545 . . . ?
O22 Bi4 O2 Bi2 162.9(3) 3_545 . . . ?
O11 Bi4 O2 Bi2 -149.8(3) . . . . ?
O11 Bi4 O2 Bi2 -19.8(5) 2_655 . . . ?
O2 Bi4 O2 Bi1 -72.7(3) 2_655 . . . ?
O3 Bi4 O2 Bi1 -1.2(3) 2_655 . . . ?
O3 Bi4 O2 Bi1 -144.9(4) . . . . ?
O22 Bi4 O2 Bi1 147.1(3) 4_545 . . . ?
O22 Bi4 O2 Bi1 17.3(6) 3_545 . . . ?
O11 Bi4 O2 Bi1 64.6(3) . . . . ?
O11 Bi4 O2 Bi1 -165.4(2) 2_655 . . . ?
O4 Bi2 O2 Bi4 -162.8(4) . . . . ?
O1 Bi2 O2 Bi4 -71.4(4) 2_655 . . . ?
O3 Bi2 O2 Bi4 -0.7(3) . . . . ?
O6 Bi2 O2 Bi4 -139.8(3) . . . . ?
F32 Bi2 O2 Bi4 7.9(10) . . . . ?
O23 Bi2 O2 Bi4 81.7(3) 4_545 . . . ?
O12 Bi2 O2 Bi4 137.1(3) 4 . . . ?
O4 Bi2 O2 Bi1 -14.4(2) . . . . ?
O1 Bi2 O2 Bi1 76.9(3) 2_655 . . . ?
O3 Bi2 O2 Bi1 147.6(3) . . . . ?
O6 Bi2 O2 Bi1 8.6(4) . . . . ?
F32 Bi2 O2 Bi1 156.2(8) . . . . ?
O23 Bi2 O2 Bi1 -130.0(3) 4_545 . . . ?
O12 Bi2 O2 Bi1 -74.5(3) 4 . . . ?
O1 Bi1 O2 Bi4 72.2(3) . . . . ?
O4 Bi1 O2 Bi4 163.1(4) . . . . ?
O5 Bi1 O2 Bi4 139.1(3) . . . . ?
O3 Bi1 O2 Bi4 1.1(3) 2_655 . . . ?
O32 Bi1 O2 Bi4 -9.4(9) 2_655 . . . ?
O21 Bi1 O2 Bi4 -135.2(3) . . . . ?
O13 Bi1 O2 Bi4 -80.8(3) . . . . ?
O1 Bi1 O2 Bi2 -76.5(3) . . . . ?
O4 Bi1 O2 Bi2 14.4(2) . . . . ?
O5 Bi1 O2 Bi2 -9.6(4) . . . . ?
O3 Bi1 O2 Bi2 -147.6(3) 2_655 . . . ?
O32 Bi1 O2 Bi2 -158.1(7) 2_655 . . . ?
O21 Bi1 O2 Bi2 76.1(3) . . . . ?
O13 Bi1 O2 Bi2 130.5(3) . . . . ?
O2 Bi4 O3 Bi2 -96.2(3) 2_655 . . . ?
O2 Bi4 O3 Bi2 -0.5(2) . . . . ?
O3 Bi4 O3 Bi2 -48.48(14) 2_655 . . . ?
O22 Bi4 O3 Bi2 96.4(2) 4_545 . . . ?
O22 Bi4 O3 Bi2 -160.9(3) 3_545 . . . ?
O11 Bi4 O3 Bi2 64.0(5) . . . . ?
O11 Bi4 O3 Bi2 164.5(3) 2_655 . . . ?
O2 Bi4 O3 Bi1 0.9(2) 2_655 . . 2_655 ?
O2 Bi4 O3 Bi1 96.6(3) . . . 2_655 ?
O3 Bi4 O3 Bi1 48.63(14) 2_655 . . 2_655 ?
O22 Bi4 O3 Bi1 -166.5(3) 4_545 . . 2_655 ?
O22 Bi4 O3 Bi1 -63.8(4) 3_545 . . 2_655 ?
O11 Bi4 O3 Bi1 161.1(3) . . . 2_655 ?
O11 Bi4 O3 Bi1 -98.4(2) 2_655 . . 2_655 ?
O2 Bi2 O3 Bi4 0.5(2) . . . . ?
O4 Bi2 O3 Bi4 23.4(4) . . . . ?
O1 Bi2 O3 Bi4 99.9(3) 2_655 . . . ?
O6 Bi2 O3 Bi4 130.4(3) . . . . ?
F32 Bi2 O3 Bi4 -175.1(5) . . . . ?
O23 Bi2 O3 Bi4 -75.3(3) 4_545 . . . ?
O12 Bi2 O3 Bi4 -85.0(4) 4 . . . ?
O2 Bi2 O3 Bi1 -99.9(3) . . . 2_655 ?
O4 Bi2 O3 Bi1 -77.1(4) . . . 2_655 ?
O1 Bi2 O3 Bi1 -0.6(2) 2_655 . . 2_655 ?
O6 Bi2 O3 Bi1 29.9(5) . . . 2_655 ?
F32 Bi2 O3 Bi1 84.5(4) . . . 2_655 ?
O23 Bi2 O3 Bi1 -175.7(3) 4_545 . . 2_655 ?
O12 Bi2 O3 Bi1 174.5(3) 4 . . 2_655 ?
O7 Bi5 O4 Bi2 -72.0(4) . . . . ?
O6 Bi5 O4 Bi2 0.1(3) . . . . ?
O5 Bi5 O4 Bi2 -143.0(4) . . . . ?
O12 Bi5 O4 Bi2 -163.4(2) 1_565 . . . ?
O23 Bi5 O4 Bi2 150.0(4) . . . . ?
Bi3 Bi5 O4 Bi2 -42.8(3) . . . . ?
Bi3 Bi5 O4 Bi2 -101.1(3) 2_655 . . . ?
O7 Bi5 O4 Bi1 71.9(4) . . . . ?
O6 Bi5 O4 Bi1 144.0(4) . . . . ?
O5 Bi5 O4 Bi1 0.9(3) . . . . ?
O12 Bi5 O4 Bi1 -19.5(5) 1_565 . . . ?
O23 Bi5 O4 Bi1 -66.1(3) . . . . ?
Bi3 Bi5 O4 Bi1 101.1(3) . . . . ?
Bi3 Bi5 O4 Bi1 42.7(3) 2_655 . . . ?
O2 Bi2 O4 Bi5 161.6(4) . . . . ?
O1 Bi2 O4 Bi5 70.4(4) 2_655 . . . ?
O3 Bi2 O4 Bi5 138.9(3) . . . . ?
O6 Bi2 O4 Bi5 -0.1(3) . . . . ?
F32 Bi2 O4 Bi5 -10.8(8) . . . . ?
O23 Bi2 O4 Bi5 -135.5(3) 4_545 . . . ?
O12 Bi2 O4 Bi5 -82.8(4) 4 . . . ?
O2 Bi2 O4 Bi1 14.3(2) . . . . ?
O1 Bi2 O4 Bi1 -76.9(3) 2_655 . . . ?
O3 Bi2 O4 Bi1 -8.4(4) . . . . ?
O6 Bi2 O4 Bi1 -147.4(3) . . . . ?
F32 Bi2 O4 Bi1 -158.1(6) . . . . ?
O23 Bi2 O4 Bi1 77.2(3) 4_545 . . . ?
O12 Bi2 O4 Bi1 129.9(3) 4 . . . ?
O1 Bi1 O4 Bi5 -70.6(4) . . . . ?
O2 Bi1 O4 Bi5 -161.5(4) . . . . ?
O5 Bi1 O4 Bi5 -0.9(3) . . . . ?
O3 Bi1 O4 Bi5 -139.0(3) 2_655 . . . ?
O32 Bi1 O4 Bi5 11.0(9) 2_655 . . . ?
O21 Bi1 O4 Bi5 81.8(3) . . . . ?
O13 Bi1 O4 Bi5 135.8(3) . . . . ?
O1 Bi1 O4 Bi2 76.7(3) . . . . ?
O2 Bi1 O4 Bi2 -14.2(2) . . . . ?
O5 Bi1 O4 Bi2 146.5(3) . . . . ?
O3 Bi1 O4 Bi2 8.4(4) 2_655 . . . ?
O32 Bi1 O4 Bi2 158.4(7) 2_655 . . . ?
O21 Bi1 O4 Bi2 -130.8(3) . . . . ?
O13 Bi1 O4 Bi2 -76.8(3) . . . . ?
O4 Bi5 O5 Bi3 97.5(3) . . . 2_655 ?
O7 Bi5 O5 Bi3 0.5(2) . . . 2_655 ?
O6 Bi5 O5 Bi3 48.5(4) . . . 2_655 ?
O12 Bi5 O5 Bi3 -96.2(2) 1_565 . . 2_655 ?
O23 Bi5 O5 Bi3 -164.5(3) . . . 2_655 ?
Bi3 Bi5 O5 Bi3 18.13(19) . . . 2_655 ?
O4 Bi5 O5 Bi1 -0.7(2) . . . . ?
O7 Bi5 O5 Bi1 -97.6(3) . . . . ?
O6 Bi5 O5 Bi1 -49.6(4) . . . . ?
O12 Bi5 O5 Bi1 165.7(3) 1_565 . . . ?
O23 Bi5 O5 Bi1 97.3(2) . . . . ?
Bi3 Bi5 O5 Bi1 -80.04(17) . . . . ?
Bi3 Bi5 O5 Bi1 -98.2(3) 2_655 . . . ?
O1 Bi1 O5 Bi5 100.0(3) . . . . ?
O2 Bi1 O5 Bi5 24.6(3) . . . . ?
O4 Bi1 O5 Bi5 0.7(2) . . . . ?
O3 Bi1 O5 Bi5 129.7(3) 2_655 . . . ?
O32 Bi1 O5 Bi5 -172.6(5) 2_655 . . . ?
O21 Bi1 O5 Bi5 -74.6(2) . . . . ?
O13 Bi1 O5 Bi5 -87.8(4) . . . . ?
O1 Bi1 O5 Bi3 -0.7(2) . . . 2_655 ?
O2 Bi1 O5 Bi3 -76.0(3) . . . 2_655 ?
O4 Bi1 O5 Bi3 -100.0(3) . . . 2_655 ?
O3 Bi1 O5 Bi3 29.0(5) 2_655 . . 2_655 ?
O32 Bi1 O5 Bi3 86.7(5) 2_655 . . 2_655 ?
O21 Bi1 O5 Bi3 -175.3(3) . . . 2_655 ?
O13 Bi1 O5 Bi3 171.5(3) . . . 2_655 ?
O4 Bi5 O6 Bi3 -96.5(3) . . . . ?
O7 Bi5 O6 Bi3 -0.1(2) . . . . ?
O5 Bi5 O6 Bi3 -47.8(4) . . . . ?
O12 Bi5 O6 Bi3 65.7(4) 1_565 . . . ?
O23 Bi5 O6 Bi3 -161.5(3) . . . . ?
Bi3 Bi5 O6 Bi3 -17.5(2) 2_655 . . . ?
O4 Bi5 O6 Bi2 -0.1(2) . . . . ?
O7 Bi5 O6 Bi2 96.3(3) . . . . ?
O5 Bi5 O6 Bi2 48.7(4) . . . . ?
O12 Bi5 O6 Bi2 162.1(2) 1_565 . . . ?
O23 Bi5 O6 Bi2 -65.0(4) . . . . ?
Bi3 Bi5 O6 Bi2 96.4(3) . . . . ?
Bi3 Bi5 O6 Bi2 78.98(17) 2_655 . . . ?
O1 Bi3 O6 Bi5 99.3(3) 2_655 . . . ?
O7 Bi3 O6 Bi5 22.5(4) 2_655 . . . ?
O7 Bi3 O6 Bi5 0.1(2) . . . . ?
O5 Bi3 O6 Bi5 129.9(3) 2_655 . . . ?
O31 Bi3 O6 Bi5 -177.7(4) . . . . ?
O11 Bi3 O6 Bi5 -87.3(4) 2_665 . . . ?
O22 Bi3 O6 Bi5 -72.7(3) 4 . . . ?
O1 Bi3 O6 Bi2 -0.4(2) 2_655 . . . ?
O7 Bi3 O6 Bi2 -77.2(3) 2_655 . . . ?
O7 Bi3 O6 Bi2 -99.6(3) . . . . ?
O5 Bi3 O6 Bi2 30.2(5) 2_655 . . . ?
O31 Bi3 O6 Bi2 82.7(4) . . . . ?
O11 Bi3 O6 Bi2 173.0(3) 2_665 . . . ?
O22 Bi3 O6 Bi2 -172.4(3) 4 . . . ?
O2 Bi2 O6 Bi5 -23.1(4) . . . . ?
O4 Bi2 O6 Bi5 0.1(2) . . . . ?
O1 Bi2 O6 Bi5 -99.6(3) 2_655 . . . ?
O3 Bi2 O6 Bi5 -130.1(3) . . . . ?
F32 Bi2 O6 Bi5 173.2(4) . . . . ?
O23 Bi2 O6 Bi5 88.3(4) 4_545 . . . ?
O12 Bi2 O6 Bi5 72.9(3) 4 . . . ?
O2 Bi2 O6 Bi3 76.8(3) . . . . ?
O4 Bi2 O6 Bi3 100.0(3) . . . . ?
O1 Bi2 O6 Bi3 0.4(2) 2_655 . . . ?
O3 Bi2 O6 Bi3 -30.2(5) . . . . ?
F32 Bi2 O6 Bi3 -86.8(4) . . . . ?
O23 Bi2 O6 Bi3 -171.7(3) 4_545 . . . ?
O12 Bi2 O6 Bi3 172.8(3) 4 . . . ?
O4 Bi5 O7 Bi3 -72.2(4) . . . 2_655 ?
O6 Bi5 O7 Bi3 -144.4(4) . . . 2_655 ?
O5 Bi5 O7 Bi3 -0.7(3) . . . 2_655 ?
O12 Bi5 O7 Bi3 68.4(4) 1_565 . . 2_655 ?
O23 Bi5 O7 Bi3 20.3(5) . . . 2_655 ?
Bi3 Bi5 O7 Bi3 -144.5(6) . . . 2_655 ?
O4 Bi5 O7 Bi3 72.3(4) . . . . ?
O6 Bi5 O7 Bi3 0.1(3) . . . . ?
O5 Bi5 O7 Bi3 143.8(4) . . . . ?
O12 Bi5 O7 Bi3 -147.1(4) 1_565 . . . ?
O23 Bi5 O7 Bi3 164.8(2) . . . . ?
Bi3 Bi5 O7 Bi3 144.5(6) 2_655 . . . ?
O1 Bi3 O7 Bi5 -71.2(3) 2_655 . . . ?
O7 Bi3 O7 Bi5 -162.3(2) 2_655 . . . ?
O5 Bi3 O7 Bi5 -139.0(3) 2_655 . . . ?
O6 Bi3 O7 Bi5 -0.1(3) . . . . ?
O31 Bi3 O7 Bi5 4.0(9) . . . . ?
O11 Bi3 O7 Bi5 134.9(3) 2_665 . . . ?
O22 Bi3 O7 Bi5 82.6(4) 4 . . . ?
O1 Bi3 O7 Bi3 76.5(3) 2_655 . . 2_655 ?
O7 Bi3 O7 Bi3 -14.5(4) 2_655 . . 2_655 ?
O5 Bi3 O7 Bi3 8.8(4) 2_655 . . 2_655 ?
O6 Bi3 O7 Bi3 147.6(3) . . . 2_655 ?
O31 Bi3 O7 Bi3 151.8(7) . . . 2_655 ?
O11 Bi3 O7 Bi3 -77.3(3) 2_665 . . 2_655 ?
O22 Bi3 O7 Bi3 -129.6(3) 4 . . 2_655 ?
O12 S1 O11 Bi3 -30.7(9) . . . 2_645 ?
O13 S1 O11 Bi3 -167.4(6) . . . 2_645 ?
C1 S1 O11 Bi3 79.3(9) . . . 2_645 ?
O12 S1 O11 Bi4 111.1(6) . . . . ?
O13 S1 O11 Bi4 -25.6(7) . . . . ?
C1 S1 O11 Bi4 -138.9(6) . . . . ?
O2 Bi4 O11 S1 105.2(5) 2_655 . . . ?
O2 Bi4 O11 S1 13.1(5) . . . . ?
O3 Bi4 O11 S1 83.9(5) 2_655 . . . ?
O3 Bi4 O11 S1 -46.3(7) . . . . ?
O22 Bi4 O11 S1 -76.6(5) 4_545 . . . ?
O22 Bi4 O11 S1 161.2(6) 3_545 . . . ?
O11 Bi4 O11 S1 -132.1(6) 2_655 . . . ?
O2 Bi4 O11 Bi3 -101.6(3) 2_655 . . 2_645 ?
O2 Bi4 O11 Bi3 166.3(3) . . . 2_645 ?
O3 Bi4 O11 Bi3 -122.8(3) 2_655 . . 2_645 ?
O3 Bi4 O11 Bi3 106.9(4) . . . 2_645 ?
O22 Bi4 O11 Bi3 76.6(2) 4_545 . . 2_645 ?
O22 Bi4 O11 Bi3 -45.6(2) 3_545 . . 2_645 ?
O11 Bi4 O11 Bi3 21.13(10) 2_655 . . 2_645 ?
O12 S1 C1 F13 58.9(13) . . . . ?
O13 S1 C1 F13 177.3(12) . . . . ?
O11 S1 C1 F13 -60.7(13) . . . . ?
O12 S1 C1 F12 177.3(11) . . . . ?
O13 S1 C1 F12 -64.3(12) . . . . ?
O11 S1 C1 F12 57.7(13) . . . . ?
O12 S1 C1 F11 -64.6(12) . . . . ?
O13 S1 C1 F11 53.9(12) . . . . ?
O11 S1 C1 F11 175.8(10) . . . . ?
O22 S2 C2 F22 -176.2(12) . . . . ?
O23 S2 C2 F22 -57.3(13) . . . . ?
O21 S2 C2 F22 64.3(14) . . . . ?
O22 S2 C2 F23 65.3(13) . . . . ?
O23 S2 C2 F23 -175.8(12) . . . . ?
O21 S2 C2 F23 -54.3(14) . . . . ?
O22 S2 C2 F21 -55.4(13) . . . . ?
O23 S2 C2 F21 63.5(13) . . . . ?
O21 S2 C2 F21 -174.9(12) . . . . ?
O33 S3 C3 F33 66(2) . . . . ?
O32 S3 C3 F33 -55(2) . . . . ?
O31 S3 C3 F33 -175(2) . . . . ?
O33 S3 C3 F32 -176.8(18) . . . . ?
O32 S3 C3 F32 61.8(19) . . . . ?
O31 S3 C3 F32 -57.4(18) . . . . ?
O33 S3 C3 F31 -62(2) . . . . ?
O32 S3 C3 F31 176.2(17) . . . . ?
O31 S3 C3 F31 56.9(17) . . . . ?
